Structural Features of Sm- and Gd-Doped Ceria Studied by Synchrotron X-ray Diffraction and μ-Raman Spectroscopy.
Artini, Cristina; Pani, Marcella; Carnasciali, Maria Maddalena; Buscaglia, Maria Teresa; Plaisier, Jasper Rikkert; Costa, Giorgio Andrea; Inorganic chemistry 54 (2015) 4126–4137; doi:10.1021/acs.inorgchem.5b00395

data_4343144
_publ_section_title
;
 Structural Features of Sm- and Gd-Doped Ceria Studied by Synchrotron
 X-ray Diffraction and \m-Raman Spectroscopy.
;
_journal_issue                   8
_journal_name_full               'Inorganic chemistry'
_journal_page_first              4126
_journal_page_last               4137
_journal_paper_doi               10.1021/acs.inorgchem.5b00395
_journal_volume                  54
_journal_year                    2015
_chemical_formula_sum            'Ce0.6 O1.8 Sm0.4'
_chemical_formula_weight         173.0120
_chemical_name_common            'Cerium samarium mixed oxide'
_space_group_IT_number           206
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-I 2b 2c 3'
_symmetry_space_group_name_H-M   'I a -3'
_cell_angle_alpha                90.00000
_cell_angle_beta                 90.00000
_cell_angle_gamma                90.00000
_cell_formula_units_Z            32
_cell_length_a                   10.89875(6)
_cell_length_b                   10.89875(6)
_cell_length_c                   10.89875(6)
_cell_measurement_temperature    298
_cell_volume                     1294.584(12)
_computing_structure_refinement  FULLPROF
_diffrn_ambient_temperature      295
_diffrn_detector                 'fast scintillator detector'
_diffrn_measurement_device_type  'Huber 4-axes X-ray diffractometer'
_diffrn_measurement_method       '2\q in the range 5-60 deg'
_diffrn_radiation_wavelength     0.74923
_diffrn_source                   synchrotron
_exptl_absorpt_coefficient_mu    41.16
_exptl_absorpt_correction_type   none
_pd_char_colour                  white
_pd_instr_location
; powder diffraction beamline (MCX) of the Elettra synchrotron radiation
 facility located in Trieste, Italy
;
_pd_meas_2theta_range_inc        0.010000
_pd_meas_2theta_range_max        80.00000
_pd_meas_2theta_range_min        9.00000
_pd_meas_number_of_points        7101
_pd_meas_scan_method             step
_pd_prep_pressure                101
_pd_prep_temperature             1473
_pd_proc_2theta_range_inc        0.010000
_pd_proc_2theta_range_max        80.0000
_pd_proc_2theta_range_min        9.0000
_pd_proc_ls_background_function
;
linear interpolation between a set of background points with refinable heights
;
_pd_proc_ls_profile_function     Pseudo-Voigt
_pd_proc_ls_prof_R_factor        6.6280
_pd_proc_ls_prof_wR_expected     5.5533
_pd_proc_ls_prof_wR_factor       8.7289
_pd_proc_wavelength              0.749230
_pd_spec_mounting
' quartz capillary tube with inner diameter of 0.5 mm '
_pd_spec_mount_mode              transmission
_pd_spec_shape                   cylinder
_pd_spec_size_axial              20
_pd_spec_size_equat              0.5
_refine_ls_goodness_of_fit_all   1.57
_refine_ls_number_parameters     106
_refine_ls_number_reflns         599
_refine_ls_number_restraints     0
_refine_ls_R_I_factor            3.6655
_refine_ls_shift/su_max          0.1
_cod_data_source_file            ic5b00395_si_002.cif
_cod_data_source_block           Sm40_1473
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Cubic' changed to 'cubic' according
to
/usr/data/users/saulius/crontab/automatic-downloads/current/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 3271 2015-04-21 07:52:19Z andrius 
;
_cod_original_cell_volume        1294.582(13)
_cod_original_formula_sum        'Ce0.6  O1.8 Sm0.4'
_cod_database_code               4343144
_pd_proc_ls_prof_cr_factor       21.2386
_pd_proc_ls_prof_cwr_factor      17.3383
_pd_proc_ls_prof_cwr_expected    11.0305
_pd_proc_ls_prof_chi2            2.4707
_pd_proc_ls_prof_echi2           2.5358